Figure 1 - uploaded by Carolin Schmitz-Antoniak
Content may be subject to copyright.

# Schematic illustration of top down and bottom up methods for the preparation of nanoparticles.

Source publication
Article
Full-text available
X-ray absorption spectroscopy facilitated by state-of-the-art synchrotron radiation technology is presented as a powerful tool to study nanoscale systems, in particular revealing their static element-specific magnetic and electronic properties on a microscopic level. A survey is given on the properties of nanoparticles, nanocomposites and thin film...

## Contexts in source publication

Context 1
... the preparation of nanoscale systems, different approaches are pursued that can be classified as top down and bottom up methods, respectively, as depicted in figure 1. The former describes the division of a massive solid into smaller portions e.g. by the use of lithographic patterning or milling. ...
Context 2
... it is common to measure the x-ray absorption related to core-level electron excitations from 2p 3/2 and 2p 1/2 states into the 3d states (so- called L 3 and L 2 absorption edges, respectively). Electronic transitions into higher unoccupied states or even into the con- tinuum are separated by a two-step-like function from the transitions into the 3d states as shown in figure 10. The height for these two steps reflects the occupation of initial states that is two times higher for the 2p 3/2 states than for the 2p 1/2 states. ...
Context 3
... oscillatory behaviour in the extended energy range about 100-1000 eV above the absorption edge, is visible in the absorption signal as can be seen in figure 11. In a simple pic- ture, these oscillations are caused by an interference effect between the outgoing photoelectron as a matter wave and backscattered waves from neighbouring atoms. ...
Context 4
... the point of the matter is that in the k-dependence of EXAFS amplitudes, important infor- mation of the type of backscattering atom is included. In figure 12, the Fourier transform and the wavelet transform are shown exemplarily for the EXAFS data presented in fig- ure 11. However the potential to directly visualise contribu- tions of different elemental species is not obvious here, but becomes evident in the example presented in the following subsection. ...
Context 5
... the point of the matter is that in the k-dependence of EXAFS amplitudes, important infor- mation of the type of backscattering atom is included. In figure 12, the Fourier transform and the wavelet transform are shown exemplarily for the EXAFS data presented in fig- ure 11. However the potential to directly visualise contribu- tions of different elemental species is not obvious here, but becomes evident in the example presented in the following subsection. ...
Context 6
... the following, the main results and conclusions are summarised from the perspective of x-ray absorption. In figure 13 the magnitudes of the FT and the WT are shown for Fe nanopar- ticles synthesised using 2 equivalent diisopropylamine-borane (AeB) as a reducing agent. In this reaction, the reduction of the Fe precursor is accompanied by the reaction of AeB to amino borane (AoB)-containing a BH 2 group instead of the BH 3 in AeB-and H 2 as depicted in figure 14. ...
Context 7
... figure 13 the magnitudes of the FT and the WT are shown for Fe nanopar- ticles synthesised using 2 equivalent diisopropylamine-borane (AeB) as a reducing agent. In this reaction, the reduction of the Fe precursor is accompanied by the reaction of AeB to amino borane (AoB)-containing a BH 2 group instead of the BH 3 in AeB-and H 2 as depicted in figure 14. In the total WT ( figure 13(b)), three peaks are clearly vis- ible: one at a radial distance of about 0.14 nm and a wavenum- ber of about 20 nm −1 , the second one at the same wavenumber, but larger radial distance (about 0.21 nm) and the third one at a radial distance of about 0.2 nm and a significantly higher wavenumber of about 60 nm −1 . ...
Context 8
... this reaction, the reduction of the Fe precursor is accompanied by the reaction of AeB to amino borane (AoB)-containing a BH 2 group instead of the BH 3 in AeB-and H 2 as depicted in figure 14. In the total WT ( figure 13(b)), three peaks are clearly vis- ible: one at a radial distance of about 0.14 nm and a wavenum- ber of about 20 nm −1 , the second one at the same wavenumber, but larger radial distance (about 0.21 nm) and the third one at a radial distance of about 0.2 nm and a significantly higher wavenumber of about 60 nm −1 . As a reference system, Fe nanoparticles synthesised by hydrogenation without any fur- ther reducing agent were measured yielding the WT shown in figure 13(c). ...
Context 9
... the total WT ( figure 13(b)), three peaks are clearly vis- ible: one at a radial distance of about 0.14 nm and a wavenum- ber of about 20 nm −1 , the second one at the same wavenumber, but larger radial distance (about 0.21 nm) and the third one at a radial distance of about 0.2 nm and a significantly higher wavenumber of about 60 nm −1 . As a reference system, Fe nanoparticles synthesised by hydrogenation without any fur- ther reducing agent were measured yielding the WT shown in figure 13(c). Only one peak is obtained that can be assigned to Fe and possible traces of other light elements like oxygen and/ or nitrogen present in the Fe precursor. ...
Context 10
... one peak is obtained that can be assigned to Fe and possible traces of other light elements like oxygen and/ or nitrogen present in the Fe precursor. After subtraction of the reference signal, the typical fingerprint of boron is obtained in figure 13(d). ...
Context 11
... less AeB as reducing agent for the synthe- sis of Fe nanoparticles leads to less boron incorporated. From the reaction scheme ( figure 14) it is evident that the boron incorporation occured in the second reaction step of the AoB byproduct connected to a further release of H 2 . To gain more insight into the chemical reaction, pre-formed Fe nanoparti- cles prepared by hydrogenation (without any boron) were sub- sequently mixed with AeB at room temperature. ...
Context 12
... gain more insight into the chemical reaction, pre-formed Fe nanoparti- cles prepared by hydrogenation (without any boron) were sub- sequently mixed with AeB at room temperature. As described in [145], a fast H 2 evolution was observed evidencing the effi- ciency of these Fe nanoparticles for dehydrogenation of AeB, as depicted in figure 15, step 1. However, the reactivity does not stop with the release of AoB, as incorporation of boron step 2 is revealed from EXAFS measurements. ...
Context 13
... a second experiment, AoB was reacted with the preformed Fe nanopar- ticles. Here again, H 2 evolution was observed, thus evidencing the activity of the Fe nanoparticles towards dehydrogenation of the AoB moiety ( figure 15, step 2). The proof of boron incorporation in Fe nanoparticles studied in this work by EXAFS analysis opens a route for the preparation of Fe-B nanoparticles and reveals the property of Fe nanoparticles to dehydrogenate both AeB and AoB derivatives. ...
Context 14
... 3 O 4 crystallises in an inverse spinel structure that is depicted in figure 16 ...
Context 15
... we pres- ent some multiplet calculation results using the CTM4XAS programme [147] which offers the possibility to calculate the different contributions of different Fe ions to the overall XANES signal site-and valence-specifically. The contribu- tions are shown in figure 17 for Fe 3+ at either O h or tetrahe- dral T d sites and Fe 2+ at O h sites. The crystal field parameters describing the influence of the surrounding oxygen ions were set to 10Dq = 1.5 eV for O h sites and 10Dq = 0.7 eV for T d sites, respectively as suggested in the literature [148,149]. ...
Context 16
... spectra were calculated with a Lorentzian broadening of 0.25 eV and a Gaussian broadening of 0.3 eV to account for lifetime effects and finite energy resolution in experiments. It can clearly be seen that the spectral shape for Fe 2+ figure 17, there may be two reasons for the occurrence of a pre-peak feature in the XANES: Fe 2+ ions and Fe 3+ on octahedral sites. The latter yields only a small pre-peak compared to the intensity of the main peak, whereas Fe 2+ yields a more pronounced pre-peak. ...
Context 17
... after three days stored in a sealed glass bottle, the Fe 2+ fraction is significantly reduced indicating a fur- ther oxidation of Fe 3 O 4 towards γ-Fe 2 O 3 . Exposure to air gives rise to an even faster oxidation of Fe 3 O 4 nanoparticles in dispersion which is shown in figure 18. These measure- ments have been performed at the HZB-BESSYII synchro- tron radiation facility using the Liquidrom endstation at the U41-PGM beamline. ...
Context 18
... addition, Al as a light element produces only a weak background of secondary electrons and, thus, a clear total electron yield signal from the underlying element can be detected. Figure 19 shows a scanning electron microscopy image of FePt nanoparticles with a mean diameter of about 6 nm deposited onto a natu- rally oxidised Si wafer using the spin-coating technique. The particles were synthesised following the wet-chemical route reported by Sun et al [150]. ...
Context 19
... the simulations clusters of chemically ordered FePt cuboctahedra covered by a layer of Al, Cu or Au were mod- elled and the system was allowed to relax structurally [35]. The results are visualised in figure 21. It can clearly be seen that capping with Al has a strong influence on the morphology of the nanoparticle, while the structural modifications for Au or Cu capping are only moderate. ...

## Similar publications

Article
Full-text available
Hagi ware originally consists of a mixture of two raw materials: Daido clay and Mishima clay. During its firing process, we observed a change in the magnetic properties of the iron oxide, Fe2O3. The magnetic moment of the Daido clay (which only contains a small amount of the Fe2O3 γ-phase) attains a maximum at a firing temperature of approximately...
Article
Full-text available
The engineering of materials with controlled magnetic properties by means other than a magnetic field is of great interest in nanotechnology. In this study, we report engineered magnetic graphene oxide (MGO) in the nanocomposite form of iron oxide nanoparticles (IO)-graphene oxide (GO) with tunable core magnetism and magnetic resonance transverse r...
Article
Full-text available
The study of the influence of the size of magnetite and maghemite clusters on the magnetic properties (magnetic moment and the Curie temperature, the blocking temperature, etc.) is performed. For separating by size, the magnetic separation and centrifugation of the aqueous solution of iron oxide nanoparticles were applied. Native particles and the...

## Citations

... Magnetic anisotropy energy (MAE) dependence on particle's volume leads to superparamagnetic effect due to which magnetisation starts fluctuating. The temperature at which magnetisation fluctuation occurs is called blocking temperature [5]. Literatures do not provide any standard procedure to deduce blocking temperature for nanoparticles. ...
... Literatures do not provide any standard procedure to deduce blocking temperature for nanoparticles. Antoniak [5] referred inflection point temperature in ZFC as the θB. Presa et al. [6] represented temperature corresponding to maximum ZFC magnetization as θB for γ-Fe2O3 nanoparticles. ...
... By sliding the magnetic arrays against each other, different types of linear and circular polarization can be obtained. Figure adapted from[142]. ...
Thesis
For more than 40 years, most astrophysical observations and laboratory studies of two key soft X-ray diagnostic 2p-3d transitions, 3C and 3D, in Fe XVII ions found oscillator-strength ratios f3C/ f3D disagreeing with theory. This discrepancy hampered the proposed plasma diagnostic utility based on the observed intensity ratios ever since. In previous laboratory measurements, the ratio was determined by scrutinizing the photon emission of an electron-impact excited plasma. First X-ray laser spectroscopy experiments at a free-electron laser (FEL) confirmed the discrepancy between experiments and theory independently of electron-excitation cross sections that could have falsified previous laboratory measurements. In this thesis, the 3C/3D oscillator-strength ratio was measured by resonantly exciting the transitions utilizing highly brilliant and monochromatic X-ray synchrotron light. Thereby, two proposed systematical effects that could have lowered the results of the FEL measurements were excluded. The final result f3C/ f3D = 3.51(7) of this work is in excellent agreement with the newest state-of-the-art theoretical predictions and appears to finally resolve the long-lasting conundrum. Additionally, for the first time, the individual natural linewidths of lines 3C and 3D, among others, were determined with an uncertainty of � 15%. The findings of this thesis now allow the observed intensity ratios of 3C and 3D to enable their usefulness in the diagnostics of astrophysical spectra.
... In addition, uncertain concentration, morphology and magnetization of particles, and possible chemical ageing also results in significant ambiquity. [16][17][18] Hence, it is clear that the analysis of in situ magnetization of SPION in suspensions is needed for accurately ascertaining the functionality of magnetic liquids. 5,6,14,15,[19][20][21][22][23][24] In response to these needs, several new methods based on photon scattering and resonant spectroscopies have recently been developed. ...
Article
Full-text available
We show that the properties of superparamagnetic iron oxide nanoparticles suspended in liquids can be effectively studied using Magnetic Circular Dichroism in Resonant Inelastic X-ray Scattering. Analysis of the spectral shape and magnetic contrast produced by this experiment enables an assessment of the site distribution and magnetic state of metal ions in the spinel phase. The selective magnetization profile of particles as derived from the field dependence of dichroism empowers an estimation of particle size distribution. Furthermore, the new proposed methodology discriminates sizes that are below the detection limits of X-ray and light scattering probes and that are difficult to spot in TEM.
... (a) the temperature (T B ) at which the maximum of ZFC magnetization occurs [46,47] (see also inflection-point criterion) [48] and [41,[49][50][51][52]), is already determined in Sect. 4.2 above; (b) the average blocking temperature 〈T B 〉, above which the coercive field and remanent magnetization vanish, is estimated by the expression for the temperature dependence of the coercive fields, as follows [53,54]. ...
Article
Full-text available
X-band EPR spectra on SiCN ceramics, doped with Fe(III) ions, annealed at 800 °C, 1000 °C, 1100 °C, 1285 °C, and 1400 °C have been simulated to understand better their magnetic properties, accompanied by new magnetization measurements in the temperature range of 5–400 K for zero-field cooling (ZFC) and field cooling (FC) at 100C. The EPR spectra reveal the presence of several kinds of Fe-containing nanoparticles with different magnetic properties. The maxima of the temperature variation of ZFC magnetization were exploited to estimate (i) the blocking temperature, which decreased with annealing temperature of the samples and (ii) the distribution of the size of Fe-containing nanoparticles in the various samples, which was found to become more uniform with increasing annealing temperature, implying that more homogenous magnetic SiCN/Fe composites can be fabricated by annealing at even higher temperatures than 1400 °C to be used as sensors. The hysteresis curves showed different behaviors above (superparamagnetic), below (ferromagnetic), and about (butterfly shape) the respective average blocking temperatures, 〈TB〉. An analysis of the coercive field dependence upon temperature reveals that it follows Stoner–Wohlfarth model for the SiCN/Fe samples annealed above 1100 °C, from which the blocking temperatures was also deduced.
... Due to the static magnetic field lines between the opposite magnets, the electrons are forced to follow oscillating paths and as a result, emit radiation. The interference of the radiation of different magnets results in a spectrum with quasi-monochromatic peaks [115]: ...
... circularly polarized x-rays by a shift of λ U /4. Similarly, the left circularly polarized x-rays can be tuned by a shift of −λ U /4. For details, see [113,115] and [26]. can be tuned by a grating unit via Bragg's law [41]: ...
... A fourth possible case of left circularly polarized x-ray is not shown here. Taken from[115]. ...
Thesis
This thesis deals with the magnetization dynamics in nanostructures of NiFe alloys induced by an electric current via the spin transfer torque effect (STT). Single-pulse and time-resolved experiments have been carried out, imaging the magnetic domains in a photoemission electron microscope (PEEM), using the circular polarized synchrotron radiation of BESSY-II. In single-pulse experiments, the reaction of magnetic domains and domain walls (DWs) upon individual current pulses in the nanostructures are studied and the approximate threshold current density for the domain wall motion was determined to about 7.5 x 1011 A/m2 in Ni20Fe80 nanowires. We designed three different types of nanostructures, favorable for different types of domain walls: a V-shape, a half ring-shape and a notched half ring-shape. Besides the inﬂuence of the current pulses on domain textures, we observed that high current pulses created new multiple domain configurations, like diamond patterns and domain arrays. For those, rather than nucleation due to STT, a temperature rise seems to be the dominant mechanism. We also observed the conversion from a vortex-like ﬂux closure domain into a transverse wall (TW). To enable time-resolved studies of the domain wall motion in pump-probe experiments with enough intensity, several modifications for a time-resolving mode had to be integrated into our energy filtered aberration-corrected PEEM: (1) A new modified sample holder for shorter current pulses (1 ns). (2) A negative deﬂection-gating concept to increase the intensity while discriminating the signal from all the multi-bunches (MBs) with no adjacent pump pulse. We observed reversible domain wall motion in Ni80Fe20 notched half-ring nanowire on a nanosecond (ns) timescale for the first time in a truly current-induced pump-probe experiment by an energy filtered aberration-corrected photoemission electron microscope. The setup consists of a newly modified sample holder, which enables magnetization changes in a nanowire by ns pulses. Within the sample holder, current pulses are generated by a fast avalanche photodiode and synchronized with the BESSY single-bunch clock. The x-ray magnetic circular dichroism (XMCD) signal is then probed at different time delays before, during and after the current pulse in a stroboscopic mode with circularly polarized synchrotron radiation in the energy range of the Fe L3-edge (707 eV). We obtained the oscillation frequency of 0.46 GHz for a domain wall. Comparing the results to a proposed string model, we find that domain wall oscillations are comparable with a string-like asymmetric oscillation.
... Since the tip is located in the far-field, i.e., it is not in the electron tunneling distance, the current increase is caused by the electrons emitted from an ensemble average of Co on the surface. Such current versus energy (I-E) spectroscopy is related to the X-ray-absorption cross section of the material, and it is akin to conventional X-ray absorption spectroscopy (XAS) 9,18 except that an SX-STM tip is used here as a local detector. ...
Article
Full-text available
We use a nanofabricated scanning tunneling microscope tip as a detector to investigate local X-ray induced tunneling and electron emission from a single cobalt nanocluster on a Au(111) surface. The tip-detector is positioned a few angstroms above the nanocluster, and ramping the incident X-ray energy across the Co photoabsorption K-edge enables the detection of element specific electrons. Atomic-scale spatial dependent changes in the X-ray absorption cross section are directly measured by taking the X-ray induced current as a function of X-ray energy. From the measured sample and tip currents, element specific X-ray induced current components can be separated and thereby the corresponding yields for the X-ray induced processes of the single cobalt nanocluster can be determined. The detection of element specific synchrotron X-ray induced electrons of a single nanocluster opens an avenue for materials characterization on a one particle at-a-time basis.
Article
Room temperature sodium‐sulfur (RT Na‐S) battery with high theoretical energy density and low cost has spurred tremendous interest, which is recognized as an ideal candidate for large‐scale energy storage applications. However, serious sodium polysulfide shutting and sluggish reaction kinetics lead to rapid capacity decay and poor Coulombic efficiency. Recently, catalytic materials capable of adsorbing and catalyzing the conversion of polysulfides are profiled as a promising method to improve electrochemical performance. In this review, the research progress is summarized that the application of catalytic materials in RT Na‐S battery. For the role of catalyst on the conversion of sulfur species, specific attention is focused on the influence factors of reaction rate during different redox processes. Various catalytic materials based on lightweight and high conductive carbon materials, including heteroatom‐doped carbon, metals and metal compounds, single‐atom and heterostructure, promote the reaction kinetic via lowered energy barrier and accelerated charge transfer. Additionally, the adsorption capacity of the catalytic materials is the key to the catalytic effect. Particular attention to the interaction between polysulfides and sulfur host materials is necessary for the exploration of catalytic mechanism. Lastly, the challenges and outlooks toward the desired design of efficient catalytic materials for RT Na‐S battery are discussed.
Article
Metal-sulfur batteries are recognized as a promising candidate for next generation electrochemical energy storage systems owing to their high theoretical energy density, low cost and environmental friendliness. However, sluggish redox kinetics of sulfur species and the shuttle effect lead to large polarization and severe capacity decay. Numerous approaches from physical barrier, chemical adsorption strategies to electrocatalysts have been tried to solve these issues and pushed the rate and cycle performance of sulfur electrodes to higher levels. Most recently, single-atom catalysts (SACs) with high catalytic efficiency have been introduced into metal-sulfur systems to achieve fast redox kinetics of sulfur conversion. In this review, we systematically summarize the current progress on SACs for sulfur electrodes from aspects of synthesis, characterization and electrochemical performance. Challenges and potential solutions for designing SACs for high-performance sulfur electrodes are discussed.
Chapter
Photoemission spectroscopies are experimental techniques based on the photoelectric effect, first observed by Heinrich Hertz in 1887 [1]. When light of sufficiently high frequency $$\nu$$ irradiates a metal, electrons with a maximum kinetic energy of $$E_{K}^{max}=h\nu -W$$, where W is the material work function, can be extracted. Einstein was awarded the Nobel prize for his explanation of the effect, which relies on the wave-particle duality of light. The same basic process is used in modern experiments to gain insight into the electronic structure of solids. The current of photoelectrons is related to the electronic density of states; the larger the number of electrons that leave a sample with a given kinetic energy, the larger is the density of states at the corresponding binding energy.
Article
Full-text available
There is a need for biofunctionalised magnetic nanoparticles for many biomedical applications, including MRI contrast agents that have a range of surface properties and functional groups. A library of eleven adducts, each formed by condensing a reducing sugar with a catechol hydrazide, for nanoparticle functionalisation has been created using a high-throughput chemical synthesis methodology. The enzymatic transformation of an N-acetylglucosamine (GlcNAc) adduct into an N-acetyllactosamine adduct by β-1,4-galactosyltransferase illustrates how chemoenzymatic methods could provide adducts bearing complex and expensive glycans. Superparamagnetic iron oxide nanoparticles (8 nm diameter, characterised by TEM, DLS and SQUID) were coated with these adducts and the magnetic resonance imaging (MRI) properties of GlcNAc-labelled nanoparticles were determined. This straightforward approach can produce a range of MRI contrast agents with a variety of biofunctionalised surfaces.